Highly tunable metal‒organic frameworks with open metal centers
Choi, Eun-Young; Wray, Curtis A.; Hu, Chunhua; Choe, Wonyoung; CrystEngComm 11 (2009) 553–; doi:10.1039/b819707p

data_7200659
_publ_section_title
;
 Highly tunable metal--organic frameworks with open metal centers
;
_journal_issue                   4
_journal_name_full               CrystEngComm
_journal_page_first              553
_journal_paper_doi               10.1039/b819707p
_journal_volume                  11
_journal_year                    2009
_chemical_formula_moiety         'C48 H30 N4 O11 Zn3'
_chemical_formula_sum            'C48 H30 N4 O11 Zn3'
_chemical_formula_weight         1034.87
_chemical_name_systematic
;
?
;
_space_group_IT_number           139
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXTL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   16.6940(10)
_cell_length_b                   16.6940(10)
_cell_length_c                   18.5799(15)
_cell_measurement_reflns_used    6692
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      24.92
_cell_measurement_theta_min      2.19
_cell_volume                     5178.0(6)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'Bruker SHELXTL'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker SMART APEX CCD'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0665
_diffrn_reflns_av_sigmaI/netI    0.0206
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            29596
_diffrn_reflns_theta_full        26.06
_diffrn_reflns_theta_max         26.06
_diffrn_reflns_theta_min         1.64
_diffrn_standards_decay_%        0
_exptl_absorpt_coefficient_mu    0.718
_exptl_absorpt_correction_T_max  0.9636
_exptl_absorpt_correction_T_min  0.7651
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            dark_purple
_exptl_crystal_density_diffrn    0.664
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             1048
_exptl_crystal_size_max          0.39
_exptl_crystal_size_mid          0.33
_exptl_crystal_size_min          0.05
_platon_squeeze_details
;
Disordered, independent solvent molecules were eliminated from the refinement
using SQUEEZE/PLATON [Spek, A.L. (2003), J. Appl. Cryst. 36, 7-13].

R factors before data are squeezed:
_refine_ls_R_factor_all 0.1223
_refine_ls_R_factor_gt 0.1022
_refine_ls_wR_factor_ref 0.3491
_refine_ls_wR_factor_gt 0.3232
;
_refine_diff_density_max         0.641
_refine_diff_density_min         -0.320
_refine_diff_density_rms         0.061
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.036
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     98
_refine_ls_number_reflns         1496
_refine_ls_number_restraints     10
_refine_ls_restrained_S_all      1.038
_refine_ls_R_factor_all          0.0647
_refine_ls_R_factor_gt           0.0481
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0963P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1283
_refine_ls_wR_factor_ref         0.1373
_reflns_number_gt                1195
_reflns_number_total             1496
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b819707p.txt
_cod_data_source_block           c7ch35-i4mmmsq
_cod_original_sg_symbol_Hall     '-I 4 2 '
_cod_database_code               7200659